**Cage rattling does not correlate with the local geometry in molecular liquids**

S. Bernini

*Dipartimento di Fisica “Enrico Fermi”, Universit`a di Pisa,*
*Largo B.Pontecorvo 3, I-56127 Pisa, Italy*

F. Puosi

*Laboratoire Interdisciplinaire de Physique, Universit`e Joseph Fourier Grenoble,*
*CNRS, 38402 Saint Martin d’H`eres, France*

D. Leporini∗

*Dipartimento di Fisica “Enrico Fermi”, Universit`a di Pisa,*
*Largo B.Pontecorvo 3, I-56127 Pisa, Italy and*

*IPCF-CNR, UOS Pisa, Italy*
(Dated: June 26, 2014)

### Abstract

Molecular-dynamics simulations of a liquid of short linear molecules have been performed to investigate
the correlation between the particle dynamics in the cage of the neighbors and the local geometry. The latter
is characterized in terms of the size and the asphericity of the Voronoi polyhedra. The correlation is found
**to be poor. In particular, in spite of the different Voronoi volume around the end and the inner monomers**
of a molecule, all the monomers exhibit coinciding displacement distribution when they are caged (as well
as at longer times during the structural relaxation). It is concluded that the fast dynamics during the cage
trapping is a non-local collective process involving monomers beyond the nearest neighbours.

PACS numbers:

Keywords: glass transition, molecular-dynamics simulation, local order, oligomers

**I.** **INTRODUCTION**

Global order is virtually absent in systems like glasses and liquids. On the contrary, local order
is present in both disordered and ordered phases [1–4]. A crucial aspect of the solidification
lead-ing to a glass is that it is associated only to subtle static structure changes, e.g. the static structure
factorS(q), measuring the spatial correlations of the particle positions, does not show
apprecia-ble changes on approaching the glass transition (GT). The absence of apparent static correlations
**distinguishing a glass and a liquid motivated research where the focus is on the dynamical **

**facil-itation by mobile particles on the nearby ones to trigger their kinetics [5]. The facilitation**
**approach is seen as an attempt to put in a more microscopic way the concept of free volume**
**by assuming that geometrical constraints act at the level of kinetic rules with no reference to**
**the microscopic interactions which are responsible for them [6].**

A different line of thought suggests that structural aspects matter in the dynamical behaviour of glassforming systems. This includes the Adam-Gibbs derivation of the structural relaxation [7,8] -built on the thermodynamic notion of the configurational entropy [9] -, the mode- coupling theory [10] and extensions [11], the random first-order transition theory (RFOT) [12], the frustration-based approach [13], as well as the so-called elastic models [14,15]. The search of a link between structural ordering and slow dynamics motivated several studies in liquids [16–19], colloids [20– 22] and polymeric systems [20,23–28].

On approaching the glass transition, particles are trapped by the cage of the first neighbors more effectively and the average escape time, i.e. the structural relaxation timeτα, increases from a few

picoseconds up to thousands of seconds [6,29–32]. The caged particles are not completely
immo-bilized by the surroundings but they wiggle with mean-square amplitude_{hu}2_{i on the picosecond}
time scalet⋆

. _{hu}2_{i is related to the Debye-Waller factor which, assuming harmonicity of thermal}
motion, takes the form _{exp (−q}2_{hu}2_{i/3) where q is the absolute value of the scattering vector.}
Henceforth,_{hu}2_{i will be referred to as short-time mean-square displacement (ST-MSD). The }
tem-porary trapping and subsequent escape mechanisms lead to large fluctuations around the averaged
dynamical behavior with strong heterogeneous dynamics [6] and leads to non-exponential
relax-ation and aging [33]. Despite the huge range of time scales older [34] and recent theoretical
[35–41] studies addressed the rattling process in the cage to understand the structural relaxation
- the escape process - gaining support from numerical [8, 15,41–62] and experimental works on
glassforming liquids [41,63,64] and glasses [38,65–70].

Recently, extensive molecular-dynamics (MD) simulations evidencing the universal correlation between the structural relaxation timeταandhu2i were reported in polymeric systems [52–54],

bi-nary atomic mixtures [55], colloidal gels [56] and antiplasticized polymers [41] and compared with
the experimental data concerning several glassformers in a wide fragility range (_{20 ≤ m ≤ 191)}
[52,55,57,59]. One major finding was that states with equal ST-MSD_{hu}2_{i have equal relaxation}
times τα too. For polymers states with equal ST-MSD show also equal chain reorientation rate

[53,54] and diffusivity [54]. Diffusion scaling was also observed in atomic mixtures [55]. More recently, the influence of free volume and the proper time scales to observe the genuine fast dy-namics have been considered [58, 59] as well as the breakdown of the Stokes-Einstein (SE) law [60], the relation with the elastic modulus [15] and the spatial extension of the involved particle displacements at short-times [61,62].

Insight into the scaling between relaxation and fast dynamics is provided by the particle dis-placement distribution, i.e. the incoherent, or self part, of the van Hove functionGs(r, t) [71,72].

The interpretation ofGs(r, t) is direct. The product Gs(r, t) · 4πr2dr is the probability that the

particle is at a distance between r and r + dr from the initial position after a time t. In terms of Gs(r, t) the scaling property is expressed by stating that, if two physical states, say X and Y,

*are characterized by the same displacement distribution*Gs(r, t⋆) at the rattling time t⋆, they also

*exhibit the same distribution at long times, e.g. at*τα[54,55]:

G(X)s (r, t ⋆

) = G(Y )s (r, t ⋆

) ⇐⇒ G(X)s (r, τα) = G(Y )s (r, τα) (1)

Eq.1holds even in the presence of very strong dynamical heterogeneity where both diffusive and jump-like dynamics are observed [54] and, in this respect, is consistent with previous conclusions that the long-time dynamical heterogeneity is predicted by the fast heterogeneities [47,73].

The present paper aims at investigating by molecular-dynamics (MD) simulations if the cage
dynamics on the fast time scalet⋆_{correlates with the local order in a molecular liquid. Local order}

will be characterized in terms of two measures, i.e. the volume and the asphericity of the Voronoi polyhedron (VP) surrounding a tagged particle. VP asphericity has been analyzed also in water [74–76], small molecules [77], hard spheres [78] and polymers [41,45,79,80]. For a VP withVv

volume andAvsurface the asphericity is defined as:

av =

(Av)3

36π (Vv)

2 − 1 (2)

the correlation between ST-MSD and the two measures of the local order is quite poor pointing to the non-local character of the fast motion of a particle within the cage of its neighbors.

The paper is organized as follows. In Sec. IIthe molecular model and the MD algorithms are presented. The results are discussed in Sec. III. Finally, the main conclusions are summarized in Sec. IV.

**II.** **METHODS**

Molecular-dynamics (MD) simulations of a melt of fully-flexible linear chains are performed. The interacting potential between non-bonded monomers reads as:

Up,q(r) = ε q − p p σ ∗ r q − q σ ∗ r p + Ucut (3)

Changing thep and q parameters does not affect the position r = σ∗

=√6

2 σ and the depth of the potential minimumε. The constant Ucutis chosen to ensureUp,q(r) = 0 at r ≥ 2.5 σ. Notice

thatp = 6, q = 12 yields the familiar Lennard-Jones (LJ) potential. The bonded monomers interact by a potential which is the sum of the LJ potential and the FENE (finitely extended nonlinear elastic) potential [81]: UF EN E(r) = − 1 2kR 2 0ln 1 − r 2 R2 0 (4)

wherek measures the magnitude of the interaction and R0 is the maximum elongation distance.

The parameters k and R0 have been set to 30 ε/σ2 and 1.5 σ respectively. We study systems of

about 2000 monomers at different density ρ, temperature T and p, q parameters. Each state is
labeled by the multiplet _{{ρ, p, q, T }. All quantities are in reduced units: length in units of σ,}
temperature in units of ε/kB and time in units of σpµ/ε where µ is the monomer mass. We

setµ = kB = 1. NP T and NV T ensembles have been used for equilibration runs, while NV E

ensemble has been used for production runs for a given state point (NP T : constant number of par-ticles, pres- sure and temperature;NV T : constant number of particles, volume and temperature; NV E: constant number of particles, volume and energy). NP T and NV T ensembles are stud-ied by the extended system method introduced by Andersen [82] and Nos´e [83]. The numerical integration of the augmented Hamiltonian is performed through the multiple time steps algorithm, reversible Reference System Propagator Algorithm (r-RESPA) [84]. We investigate three sets of states of a melt of trimers (M = 3):

• Set A: (1.015,7,15,1.05), (1.09,8,12,1.4) • Set B: (1.016,7,15,0.7), (1.086,6,12,0.7) • Set C: (0.984,6,12,0.33), (1.086,6,12,0.63)

The states of each set have equal ST-MSD_{hu}2_{i and structural relaxation time τ}α(see Sec.III A). In

addition we also study a melt of decamers (M = 10) with ρ = 1.086, T = 0.65 with LJ interaction between non-bonded monomers exhibiting a structural relaxation timeτα ≃ 152.

**III.** **RESULTS AND DISCUSSION**

**A.** **Correlation between cage rattling and structural relaxation**

A central quantity of interest is the distribution of the monomer displacements which is ac-counted for by the self-part of the van Hove functionGs(r, t) [71,72]:

Gs(r, t) =
1
N
* _{N}
X
i=1
δ [r + ri(0) − ri(t)]
+
(5)

In isotropic liquids, the van Hove function depends on the modulus r of r. The second moment ofGs(r, t) is related to the mean square displacement (MSD):

r2_{(t) = 4π}

Z ∞

0

r2Gs(r, t)r2dr (6)

In order to characterize the cage fast dynamics we consider the MSD evaluated at the character-istic time scalet⋆

which is defined by the condition that the derivative_{∆(t) ≡ ∂ loghr}2_{(t)i/∂ log t}
is minimum att⋆_{, i.e.}_{t}⋆ _{is the time when MSD changes the concavity in the log-log plot [}_{52}_{,}_{53}_{].}

t⋆ _{is a measure of the trapping time of the particle and corresponds to a few picoseconds in actual}

units. In the present modelt⋆

≃ 1 in MD units, irrespective of the physical state [52], and ST-MSD
is defined as_{hu}2_{i = hr}2(t = t∗

)i.

The spatial Fourier transform of the self-part of the van Hove function yields the self-part of the intermediate scattering function (ISF)Fs(q, t) [72]:

Fs(q, t) =

Z

Gs(r, t)e −iq·r

0,01 0,1 1 10 100 1000 10000 0 0,2 0,4 0,6 0,8 1

### F

s### ( q

max### , t )

0,01 0,1 1 10 100 1000 10000### t

0,001 0,01 0,1 1### < r

2### ( t ) >

10 15 20 25 30### 1

## /

### < u

2### >

0 1 2 3### Log

### τ

α A B C t* A B C A B CFIG. 1: Top: ISF of the states of the sets A,B,C; the dots mark the structural relaxation time τα. Middle:

monomer MSD of the states of the sets A,B,C._{hu}2_{i is the short-time MSD (ST-MSD) evaluated at the time}

t∗

when MSD changes the concavity in the log-log plot. Bottom: location of the sets of states in the master
curve log ταvshu2i−1 (orange line) [52]. Note that ISF and MSD of states of the same set coincide from
t_{≃ t}⋆_{onward.}

which, in an isotropic liquid, depends only on the modulus of the wavevector _{q = |q|. ISF is}
a useful tool to investigate the rearrangements of the spatial structure over the length scale 2π/q.
Since we are interested in the structural relaxation of the cage surrounding the tagged particle, ISF
is evaluated atq = qmax, where the maximum of the static structure factor is located. Accordingly,

the structural relaxation time τα is defined by the equationFs(qmax, τα) = e −1

0 0,2 0,4 0,6 0,8 0 1 2 3 4 5 6

### 4

### π

### r

2### G

s### ( r , t

*### )

0 0,5 1 1,5 2### r

0 3 6 9### 4

### π

### r

2### G

s### ( r ,

### τ

α### )

A B C A B C x2 x3 x1FIG. 2: Particle displacement distribution of the states of the sets A,B,C evaluated at the rattling time t = t∗

(top) and the structural relaxation time t = τα *(bottom). Each curve results from the virtually perfect*

superposition of the curves pertaining to the different states of each set. Note the characteristic bump at

r_{∼ 1 due to the more apparent jump dynamics occurring for the states of the C set.}

Fig.1shows ISF (top ) and MSD (middle) of the sets A,B,C. In agreement with Eqs.1,6,7, it is
seen that states with equal ST-MSD_{hu}2_{i have equal τ}α[52,54,55]. Even more, states of the same

set have coinciding MSD and ISF from times aboutt∗

onward. This points to a strong correlation between the picosecond rattling motion in the cage and the structural relaxation (the deviations in the ballistic regime at very short times are due to the different temperatures). Careful studies show that the correlation is also present in the diffusive regime, i.e. states with equal ST-MSD have equal diffusivity [54,55].

The coincidence of MSD and ISF of states with equalτα fort & t ∗

reflects the scaling of the self-part of the van Hove function, Eq.1. This is shown in Fig2which evidences the coincidence ofGs(r, t) with t = t

∗

(top) andt = τα(bottom) for states belonging to the same set. Note that the

0 0,2 0,4 0,6 0,8 0 1 2 3 4 5 6

### 4

### π

### r

2### G

s### ( r , t

*### )

Inner End 0 0,5 1 1,5 2### r

0 3 6 9### 4

### π

### r

2### G

s### ( r ,

### τ

α### )

A B C A B C x2 x3 x1 MonomerFIG. 3: Particle displacement distribution of the inner and outer monomers of the trimers for the sets of states A,B,C at the rattling time t = t∗

(top) and the structural relaxation time t = τα(bottom). For each

set of states all the curves are coinciding, namely, the displacement distribution depends on neither the monomer position along the chain nor, for a given relaxation time, the state itself.

where the characteristic bump due to the jump dynamics is apparent .

The displacement distribution in Fig.2*is averaged over all the monomers. We now prove that,*
actually, the shape of the distribution is independent of the specific monomer. To this aim, Fig.3
shows the van Hove functions of the inner and the outer monomers of the trimers for the sets of
states A,B,C. It is seen that they are virtually coincident at both short (t = t∗

) and long (t = τα)

*times and independent of the physical state for a given relaxation time.*

**B.** **Local geometry: Voronoi polyhedra**

To characterize the local geometry of the neighborhood of a tagged particle we perform a space tessellation in terms of the Voronoi polyhedra. Given a particular arrangement of the monomers,

0,7 0,8 0,9 1 1,1 1,2 1,3

### V

v 0 2 4 6 8 10### P ( V

v### )

A B C 0,3 0,35 0,4 0,45 0,5 0,55### a

v 0 3 6 9 12 15### P ( a

v### )

-2 0 2 ( V_{v}- < V

_{V}> ) · σ-1

_{V}V 0 0,25 0,5 σVV · P ( V v ) -2 0 2 ( a

_{v}- < a

_{V}> ) · σ-1

_{a}V 0 0,25 0,5 σaV · P ( a v ) Set

FIG. 4: Distribution of Voronoi polyhedra’s volume Vv (top) and asphericity av(bottom), for set A (red

**curves), B (green curves) and C (blue curves). The insets show that a single master curve is obtained**

**by shifting the distributions by the average and scaled by the root-mean-square deviation, as noted**
**before [45].**

the Voronoi polyhedron (VP) surrounding a tagged monomer encloses all the points which are closer to it than to any other one. In particular, we are interested in both their volumeVv and their

asphericityav, Eq.2.

Fig.4shows the distributions of the volume (top) and the asphericity (bottom) of the VPs for
the three sets of states under investigation. It is apparent that states of the same set do not have
the same distribution of local geometries. Remind that states belonging to the same set have
coinciding monomer displacement distribution at both short and long times (Fig.2**). The insets of**

**Fig.4show that the distributions of both the volume and the asphericity of the VPs collapse**
**to a single master curve by following Starr et al [45]. This suggests the existence of a single**
**underlying distribution.**

0,8 0,9 1 1,1 1,2 1,3

### V

v 0 2 4 6 8 10### P ( V

v### )

Inner End 0,3 0,35 0,4 0,45 0,5 0,55### a

v 0 3 6 9 12 15### P ( a

v### )

**Set C**

Monomer
FIG. 5: Distribution of the Voronoi polyhedra’s volume Vv (top) and asphericity av(bottom) for the inner

and the end monomers of the trimers of the states of the set C. Thick blue: (1.086,6,12,0.63), light blue : (0.984,6,12,0.33).

volume and the asphericity distributions of the end and the inner monomers. The results are plotted
in Fig.5**. It is seen (top panel) that end monomers have extra Voronoi volume with respect to the**
inner monomers, as it is well known since long times [85] and observed in previous MD work
[86]. Furthermore, VPs of the end monomers are more spherical. In spite of the different local
geometries around the end and the inner monomers their displacement distributions are identical
at both short and long times (Fig.3). This results is in agreement with MD studies on a 2D
**glass-forming alloy showing that having a larger Voronoi volume does not cause a particle to exhibit**
larger amplitude fluctuations in position [87].

It must be pointed out that the above results are not limited to trimers - where some correlation
between the motion of the end and the inner monomers arises from their direct bonding - but it
is also observed in longer molecules. In fact, Fig.6 shows that also in a melt of decamers the
*displacement distribution of the two end and the two innermost monomers coincide, whereas the*

0 0,2 0,4 0,6 0,8 1 1,2
r
0
1
2
3
4
5
6
4
π
r
2 G
s
( r , t )
t*
τ_{α}
0,8 0,9 1 1,1
V_{v}
0
2
4
6
8
10
P ( V
v
)
Inner
End
0,2 0,25 0,3 0,35 0,4 0,45 0,5
a_{v}
0
3
6
9
12
15
P ( a
v
)
t
**M = 10**
Monomer

FIG. 6: Dynamics and local geometry of the two end and the two innermost monomers of a single chain molecule for the melt of decamers. Top: distribution of the monomer displacements at short and long times. Notice that the displacement distributions of the end and the inner monomers are coinciding. Bottom: distributions of the VPs volume (green) and asphericity (brown).

*local geometry around them is different.*

Our findings suggest that the fast motion of a particle within the cage of the neighbors is a
non-local process. We propose that it results from the collective motion of particles in a region
extending more than the first neighbours region. In fact, equal-time, i.e. simultaneous, particle
motion correlating over the next-nearest neighbours even at the short (picosecond) time scales
has been evidenced [61, 62**]. This is consistent with the evidence of quasi-local soft modes,**

**i.e. with an extended component, in MD simulations of 2D binary mixtures and the finding**
**that the regions of motion of the quasi-local soft modes exhibit striking correlation with the**
**regions of high Debye-Waller factor [47–49].**

The conclusion that the influence of structure on dynamics is weak on short length scale has been reached before by Berthier and Jack, who predicted that it becomes much stronger on long

length scale [88]. From this respect, the evidence of strong correlations between the (long wave-length) elasticity and the fast and slow dynamics deserves further consideration [15,89].

**IV.** **CONCLUSIONS**

A supercooled liquid of linear molecules has been investigated by MD simulations. The
em-phasis is on the possible correlation between the local order and the dynamics at short and long
times, as probed by cage rattling and structural relaxation, respectively. Two measures of the local
order, i.e. the VP volume and asphericity have no clear correlation with both fast and slow
**dynam-ics. In particular, it is found that the excess Voronoi volume surrounding the end monomers does**
not enhance their dynamics neither at short nor at long times. It is concluded that fast dynamics is
a non-local process extending farther than the first neighbor shell.

**[1] P. R. ten Wolde, M. J. Ruiz-Montero, and D. Frenkel, Phys. Rev. Lett. 75, 2714 (2005).**
**[2] A. R. Kansal, S. Torquato, and F. H. Stillinger, Phys. Rev. E 66, 041109 (2002).**
**[3] T. Aste, J. Phys.: Condens. Matter 17, S2361 (2005).**

**[4] S. Bernini, F. Puosi, M. Barucco, and D. Leporini, J. Chem. Phys. 139, 184501 (2013).**
**[5] D. Chandler and J. P. Garrahan, Annu. Rev. Phys. Chem. 61, 191 (2010).**

**[6] L. Berthier and G. Biroli, Rev. Mod. Phys. 83, 587 (2011).**
**[7] G. Adam and J. H. Gibbs, J. Chem. Phys. 43, 139 (1965).**

**[8] J. Dudowicz, K. F. Freed, and J. F. Douglas, Adv. Chem. Phys. 137, 125 (2008).**
**[9] J. H. Gibbs and E. A. DiMarzio, J. Chem. Phys. 28, 373 (1958).**

*[10] W. G ¨otze, Complex Dynamics of Glass-Forming Liquids: A Mode-Coupling Theory (Oxford *
Univer-sity Press, Oxford, 2008).

**[11] K. Chen, E. J. Saltzman, and K. S. Schweizer, Annu. Rev. Condens. Matter Phys. 1, 277 (2010).**
**[12] V. Lubchenko and P. G. Wolynes, Annu. Rev. Phys. Chem. 58, 235 (2007).**

**[13] G. Tarjus, S. A. Kivelson, Z. Nussinov, and P. Viot, J. Phys.: Condens. Matter 17, R1143 (2005).**
**[14] J. C. Dyre, Rev. Mod. Phys. 78, 953 (2006).**

**[15] F. Puosi and D. Leporini, J. Chem. Phys. 136, 041104 (2012).**

**[17] S. Singh, M. D. Ediger, and J. J. de Pablo, Nat. Mater. 12, 139 (2013).**
**[18] T. Speck, A. Malins, and C. P. Royall, Phys. Rev. Lett. 109, 195703 (2012).**
**[19] A. Barbieri, G. Gorini, and D. Leporini, Phys. Rev. E 69, 061509 (2004).**
**[20] J. C. Conrad, F. W. Starr, and D. A. Weitz, J.Phys. Chem. B 109, 21235 (2005).**
**[21] C. P. Royall, S. R. Williams, T. Ohtsuka, and H. Tanaka, Nat. Mater. 7, 556 (2008).**
**[22] M. Leocmach and H. Tanaka, Nat. Commun. 3, 974 (2012).**

**[23] T. S. Jain and J. de Pablo, J.Chem.Phys. 122, 174515 (2005).**

**[24] C. R. Iacovella, A. S. Keys, M. A. Horsch, and S. C. Glotzer, Phys. Rev. E 75, 040801(R) (2007).**
**[25] N. C. Karayiannis, K. Foteinopoulou, and M. Laso, J. Chem. Phys. 130, 164908 (2009).**

**[26] B. Schnell, H. Meyer, C. Fond, J. Wittmer, and J. Baschnagel, Eur. Phys. J. E 34, 97 (2011).**
**[27] M. Asai, M. Shibayama, and Y. Koike, Macromolecules 44, 6615 (2011).**

**[28] L. Larini, A. Barbieri, D. Prevosto, P. A. Rolla, and D. Leporini, J. Phys.: Condens. Matter 17, L199**
(2005).

**[29] M. D. Ediger and P. Harrowell, J. Chem. Phys. 137, 080901 (2012).**

**[30] C. A. Angell, K. L. Ngai, G. B. McKenna, P. McMillan, and S.W.Martin, J. Appl. Phys. 88, 3113**
(2000).

**[31] P. G. Debenedetti and F. H. Stillinger, Nature 410, 259 (2001).**
**[32] R. Richert, J. Phys.: Condens. Matter 14, R703 (2002).**

**[33] C. Monthus and J.-P. Bouchaud, J. Phys. A: Math. Gen. 29, 3847 (1996).**

*[34] A. Tobolsky, R. E. Powell, and H. Eyring, in Frontiers in Chemistry, edited by R. E. Burk and*
O. Grummit (Interscience, New York, 1943), vol. 1, pp. 125–190.

**[35] C. A. Angell, Science 267, 1924 (1995).**

**[36] R. W. Hall and P. G. Wolynes, J. Chem. Phys. 86, 2943 (1987).**

**[37] J. C. Dyre, N. B. Olsen, and T. Christensen, Phys. Rev. B 53, 2171 (1996).**
**[38] L.-M. Martinez and C. A. Angell, Nature 410, 663 (2001).**

**[39] K. L. Ngai, Phil. Mag. 84, 1341 (2004).**
**[40] K. L. Ngai, J. Non-Cryst. Solids 275, 7 (2000).**

**[41] D. S. Simmons, M. T. Cicerone, Q. Zhong, M. Tyagic, and J. F. Douglas, Soft Matter 8, 11455 (2012).**
**[42] C. A. Angell, J. Am. Chem. Soc. 86, 117 (1968).**

**[43] S.V.Nemilov, Russ. J. Phys. Chem. 42, 726 (1968).**

Societ, 1995), vol. 1, pp. 311–320.

**[45] F. Starr, S. Sastry, J. F. Douglas, and S. Glotzer, Phys. Rev. Lett. 89, 125501 (2002).**
**[46] P. Bordat, F. Affouard, M. Descamps, and K. L. Ngai, Phys. Rev. Lett. 93, 105502 (2004).**
**[47] A. Widmer-Cooper and P. Harrowell, Phys. Rev. Lett. 96, 185701(4) (2006).**

**[48] A. Widmer-Cooper, H. Perry, P. Harrowell, and D. R. Reichman, Nature Physics 4, 711 (2008).**
**[49] A. Widmer-Cooper, H. Perry, P. Harrowell, and D. R. Reichman, J.Chem.Phys. 131, 194508 (2009).**
**[50] H. Zhang, D. J. Srolovitz, J. F. Douglas, and J. A. Warren, Proc. Natl. Acad. Sci. USA 106, 7735**

(2009).

**[51] X. Xia and P. G. Wolynes, PNAS 97, 2990 (2000).**

**[52] L. Larini, A. Ottochian, C. De Michele, and D. Leporini, Nature Physics 4, 42 (2008).**
**[53] A. Ottochian, C. De Michele, and D. Leporini, J. Chem. Phys. 131, 224517 (2009).**
**[54] F. Puosi and D. Leporini, J.Phys. Chem. B 115, 14046 (2011).**

**[55] F. Puosi, C. D. Michele, and D. Leporini, J. Chem. Phys. 138, 12A532 (2013).**
**[56] C. De Michele, E. Del Gado, and D. Leporini, Soft Matter 7, 4025 (2011).**

**[57] A. Ottochian, F. Puosi, C. D. Michele, and D. Leporini, Soft Matter 9, 7890 (2013).**
**[58] A. Ottochian and D. Leporini, J. Non-Cryst. Solids 357, 298 (2011).**

**[59] A. Ottochian and D. Leporini, Phil. Mag. 91, 1786 (2011).**
**[60] F. Puosi and D. Leporini, J. Chem. Phys. 136, 211101 (2012).**
**[61] F. Puosi and D. Leporini, J. Chem. Phys. 136, 164901 (2012).**
**[62] F. Puosi and D. Leporini, J. Chem. Phys. 139, 029901 (2013).**
**[63] U. Buchenau and R. Zorn, Europhys. Lett. 18, 523 (1992).**

**[64] L. Andreozzi, M. Giordano, and D. Leporini, J. Non-Cryst. Solids 235, 219 (1998).**
**[65] T. Scopigno, G. Ruocco, F. Sette, and G. Monaco, Science 302, 849 (2003).**

**[66] A. P. Sokolov, E. R ¨ossler, A. Kisliuk, and D. Quitmann, Phys. Rev. Lett. 71, 2062 (1993).**
**[67] U. Buchenau and A. Wischnewski, Phys. Rev. B 70, 092201 (2004).**

**[68] V. N. Novikov and A. P. Sokolov, Nature 431, 961 (2004).**

**[69] V. N. Novikov, Y. Ding, and A. P. Sokolov, Phys.Rev.E 71, 061501 (2005).**
**[70] S. N. Yannopoulos and G. P. Johari, Nature 442, E7 (2006).**

*[71] P. A. Egelstaff, An introduction to the liquid state (Clarendon Press, Oxford, 1992), 2nd ed.*
*[72] J. P. Hansen and I. R. McDonald, Theory of Simple Liquids, 3rd Ed. (Academic Press, 2006).*
[73] Note that t⋆is one order of magnitude shorter than the times considered in ref. [47].

**[74] P. Jedlovszky, J. Chem. Phys. 111, 5975 (1999).**

**[75] K. T. Wikfeldt, M. Leetmaa, A. Mace, A. Nilsson, and L. G. M. Pettersson, J. Chem. Phys. 132,**
104513 (2010).

**[76] G. Stirnemann and D. Laage, J. Chem. Phys. 137, 031101 (2012).**
**[77] G. Ruocco, M. Sampoli, and R. Vallauri, J. Chem. Phys. 96, 6167 (1992).**

**[78] W. P. Krekelberg, V. Ganesan, and T. M. Truskett, J. Chem. Phys. 124, 214502 (2006).**
**[79] M. Sega, P. Jedlovszky, N. N. Medvedev, and R. Vallauri, J. Chem. Phys. 121, 2422 (2004).**
**[80] D.Rigby and R. J. Roe, Macromolecules 23, 5312 (1990).**

**[81] G. S. Grest and K. Kremer, Phys. Rev. A 33, 3628 (1986).**
**[82] H. C. Andersen, J. Chem. Phys. 72, 2384 (1980).**

**[83] S. Nos´e, J. Chem. Phys. 81, 511 (1984).**

**[84] M. E. Tuckerman, B. J. Berne, and G. J. Martyna, J. Chem. Phys. 97, 1990 (1992).**
*[85] F. Bueche, Physical Properties of Polymers (Interscience, New York, 1962).*

**[86] A. Barbieri, D. Prevosto, M. Lucchesi, and D. Leporini, J. Phys.: Condens. Matter 16, 6609 (2004).**
**[87] A. Widmer-Cooper and P. Harrowell, J. Non-Cryst Solids 352, 5098 (2006).**

**[88] L. Berthier and R. L. Jack, Phys. Rev. E 76, 041509 (2007).**
[89] F.Puosi and D.Leporini, arXiv:1108.4629.